Conceptual Design of Composite Bridge Sandwich Structure

: Fiber-reinforced polymer (FRP) composite bridges are usually constructed for rapid installation. The durability of the bridge is increased by stiffness, strength to weight ratio, and corrosion resistance. The main factors on which the design of the composite sandwiched bridge considerably depends are ply layers, material system, alignment of ply angles, and thickness of the core. In this work, a parametric design study for a bridge using ﬁnite element analysis (FEA) is presented. Two types of composite materials—carbon ﬁber reinforced polymer (CFRP) and glass ﬁber reinforced polymer (GFRP)—were used as the sandwich structure’s skin, and three different types of woods were used as a core. Different design conﬁgurations were acquired based on material and instability constraints by using Euro-codes. Failure criterion of Tsai-Hill, Tsai-Wu, MS, equivalent stress, and maximum shear stress were implemented to analyze the overall failure of the bridge deck under Ultimate Limit State (ULS) conditions. The total deformation was examined under Serviceability Limit State (SLS) conditions, and the results were compared and veriﬁed by the previous study. The core was also examined using the core-factor and increasing the thickness of the core through parametric modeling.


Introduction
Fiber Reinforced Polymers (FRPs) have been widely used in marine, industrial, chemical and civil infrastructure as reinforcing and structural materials with the advantages of being lightweight, high strength, and possessing design flexibility and exceptional corrosion resistance [1][2][3]. Modern engineering systems, especially in the areas related to wind turbines [4], space [5], artery bridges [6], and marine atmospheres [7,8], gradually highlighted the importance of functional necessities. Implementing these functional requirements with materials such as concrete, conventional steel, and other similar materials possess some design challenges. Work on fiber composites with multifunctional, extraordinary-performance, and structural acclimation systems are, therefore, imperative.
A sandwich structure is a composite material structure, composed of layers and formed into a dense, lightweight core by adding two rigid, thin skins [9]. Its properties, such as a high strength-to-mass ratio and a high rigidity-to-mass bending ratio, are the most important benefits of these configurations. Due to their extraordinary resistance to corrosion, these are significantly used in aerospace and maritime systems [10][11][12]. To examine the flexural and shear behavior of layered sandwich beams (LSB), eight LSB beams made up from GFRP skins and phenolic cores were developed and tested for four-point bending and beam shear. It was examined from the FEA model that the LSB

Material Constraints
Tsai-Wu criterion is known as the most comprehensive criterion [28][29][30], since it distinguishes among a lamina's strengths both compressive and tensile and can be extended in the subsequent form SF TW ≥ 1 (1) In this work, all the values greater than 1 were considered to fulfill the Tsai-Wu criterion. The second criterion to examine the failure is Tsai-Hill (TH), denoted by SF TH [31]. There is an assumption that the material will fail when the magnitude of distortion energy is greater than the failure distortion energy of the material. It was then implemented by Tsai on the unidirectional lamina, and then he anticipated that lamina would fail if (G 2 + G 3 )σ 2 1 + (G 1 + G 3 )σ 2 2 + (G 1 + G 2 )σ 2 3 − 2G 3 σ 1 σ 2 − 2G 2 σ 1 σ 3 − 2G 1 σ 2 σ 3 + 2G 4 τ 2 23 + 2G 5 τ 2 13 + 2G 6 τ 2 12 < 1 is violated. Values of all factors are given in [12]. Both the failure criteria are called constraints for the composite material. For the safe range, both criteria must fulfill the conditions given below, and their values must be greater than 1 [12]. The third criterion implemented shows that the yield stress denoted by σ YS must be greater than the value of equivalent stress.

Instability Constraint
The deformation and core factor is used as a constraint on an instability. The core factor's values must be greater than 1 to make sure that the material is secure, and the deformation must be less than 32 mm in our case.

Structural Design (Limit State Design)
Limit State Design methodology is used to design the bridge, which is also known as LFRD (load and resistance factor design). This method is commonly used to design Appl. Sci. 2021, 11, 214 4 of 18 structures in structural engineering. A limit state is a group of performance criteria, e.g., deflection, buckling, vibration, crack width, and overall collapse, which must be met when the structure is subjected to the loadings. If the condition occurs in which the structure goes beyond the limit state, then it will not fulfill the design criteria. To ensure the safe structure and its functionality, this methodology must satisfy two criteria i.e., ULS and SLS. ULS is the computational condition according to which magnification factors are applied to the loads, and reduction factors are applied to the resistances to examine the safety of the overall structure. Whereas SLS is the computational check used to examine the deformation limits i.e., deflection, or dynamic behavior under the characteristic design loads, and thus this check is essential for all the structures, especially present in seismic areas. Through checking the (ULS) and (SLS), all bridges are built in compliance with the limit state model defined in Euro-code 2, 3 and 5 (2005). By applying the load factors to the actions and material factors to the characteristic (5 percent fractile) values, the design values of actions and properties are obtained. The variations of load and load variables have been collected from Euro-code 0 [32]. Product considerations of timber were chosen from Euro-code 5 (2005). The same material considerations were introduced for the FRP materials as in the design of the Avançon Bridge [20] based on BÜV [33] and Clarke [34]. According to Euro-code 2, at SLS conditions, the deflections for the slab and deck were limited to span/500 for short bridges [35].

Finite Element Model of the Bridge Deck
The research in this article aims to find an appropriate model for a bridge structure based on minimum mass and thickness, using natural wood and composite materials as a replacement for reinforced concrete and steel bridges. The total length and width of the bridge were taken at 16 m and 7.5 m, respectively. By fixing these both dimensions, work on different thicknesses was done. The selection of size is based on the previous study in which Balsa wood was used to design the bridge [27]. The model was created in ANSYS WORKBENCH using a geometric modeling tool for both ULS and SLS verifications. The layered shell element SHELL 181 was used in ANSYS WORKBENCH to develop the FEA model for global verification. Layered shell element has short computational time. It is easier to create the mesh in shell element, and also, it needs less disc space for results. Postprocessing in the layered shell element type is also faster. In addition, shell elements have both translations as well as rotation degrees of freedom. The main disadvantage of the solid element is locking, in which the solid element shows the bending behavior much stiffer in comparison with an analytical solution. Layered SHELL 181 is ideal for the study of thin to medium dense shell systems. This is ideally adapted for linear, broad rotation, and wide non-linear strain applications. Throughout the domain components, both complete and reduced integration schemes are supported. Layered SHELL 181 accounts for the follower (load stiffness) effects of the distributed pressure. It is a four-node feature with six degrees of freedom at each node: transformations in x, y, and z directions, and rotations in all three axes. According to the ANSYS reference manual, layered shell 181 element can be used for layered applications for modeling composite thin to moderately thick shell or sandwich structures. The accuracy of the layered shell 181 element is based on the first-order shear deformation theory (FSDT) (usually referred to as Mindlin-Reissner shell theory). In [36,37] Vrabie, used the shell element to design the sandwich structure. Moreover, according to [20], layered shell elements can be used in this type of bridge for global verification. Therefore, in the present case, the layered shell element shell 181 is expected to predict results with sufficient accuracy. For the discretization of the model, element size 0.1 m was used. The FEA model of the bridge structure used in this research is shown in Figure 1.    PrePost (ACP) module for composites of the software was used to create a preliminary model of the composite lay-up using 0.001 m of thickness. While designing the lay-up in the ACP module, Rosettes and oriented selection sets were used for fiber orientation and directions. Composite plies were then created with the help of modeling groups. Orthotropic properties were used for both wood cores and FRP skins. Boundary conditions were then applied. Displacements in the X, Y, and Z directions were constrained on both ends of the bridge, as shown in Figure 1d. A total load of running traffic on the bridge was applied in two groups, one on each lane, loads of 4 × 90 kN and 4 × 135 kN with characteristic values were applied on lane 1 and 2, respectively. In lane 1 there was a car, and a 90 kN load was applied on each wheel. The position of the car was at the center of the bridge span. The distance between the front wheels was 2 m, and the distance between the front and rear wheel was 2.   Table 2. Properties of materials used in the core of bridge [39][40][41][42][43][44].

Materials
The skin of the sandwich structure is composed of carbon/epoxy and glass/epoxy materials. The mechanical properties of these materials are shown in Table 1.
In the bridge sandwich structure, three different cores were used. The properties of the material used in the core are mentioned in Table 2. Table 3 lists the content considerations applied at ULS and SLS conditions.

Results and Discussion
All the results obtained from FEA are listed in Table 4. For each wood core, there are four cases, two for ULS and two for SLS conditions. These four cases are based upon the outer skin of CFRP and GFRP materials. Every case was composed of two laminate angle formations. Materials used in the core are shown in the first column of the Table 4. Lay-up configuration for both desired angles is mentioned in the lay-up portion. The thickness section shows the minimum values of the thickness on which the bridge is safe from all kinds of failures, both the inner and outer thicknesses are written. Total deformation is mentioned in accordance with the span limit formula in the fourth section of the table. The results of the deflection were compared with the previous study, which are the same. Please see the SU concept in [27], where for 16 m, the deformation was less than 32 mm. Michael Osei-Antwi [27] used the design methodology, which was used for experimental work by Thomas [20]. In this case, the value of deformation was less than 32 mm in each configuration. This research was extended to find six other parameters besides deflection. Different failure criteria are mentioned in the fifth section, with the minimum values on which the bridge is in stable condition. Total mass for all model configurations is then calculated and written in the last section of the column. For parametric optimization, three different types of woods were used as the core material. Cross-ply laminate [45/−45] is optimized for minimum mass and thickness on the same loading and boundary conditions. Starting from 1 mm thickness, the number of ply layers was varied to 48, and with the addition of each number, the thickness of 1 mm was increased for each ply angle to the total value. Seven different parameters were studied for the stability of the structure. Values of material constraints Tsai-Wu, Tsai-Hill, and MS should be greater than unity. The second is the deformation must be less than 32 mm according to the span limit relation span/500. All the results obtained from FEA are three are mentioned in Table 4 under ULS and SLS conditions.
For the Bamboo wood core, there were two cases for the CFRP. For ULS, the MS criterion, Tsai-Wu (SF TW ) criterion, Tsai-Hill (SF TH ) criterion and the core factor were 4.84, 4.75, 4.36, and 53.8, respectively, and were greater than 1. The fiber plies for skins were [45 10 / − 45 10 ] 20 , which showed that the total number of fiber laminates was 20 on either side with a core thickness of 400 mm. The deformation was in the safe limit, and the value was −0.032 m equals to the maximum allowable value of −0.032 m. This configuration has 43,280 kg of the total mass. The values of Equivalent stress and Maximum shear stress were 5.40 MPa, and 2.83 MPa, which were lower compared to the value of tensile strength. So, the bridge was safe in this configuration. For the ULS condition with GFRP skin, the above-stated criteria were 7.77, 7.21, 7.01, and 77.5, respectively, with the lay-up of [45 11 / − 45 11 ] 22 , and the core of 440 mm. However, the thickness and mass drastically increased to 484 mm and 50,266 kg, respectively. The deformation, in this case, was 0.028 m.
For the SLS conditions, the bamboo core and CFRP laminate skin, the MS criterion, Tsai-Wu (SF TW ) and Tsai-Hill (SF TH ) criteria and core factor were 11.26, 11.05, 10.14, and 56.59, respectively. The values of all the criteria mentioned above were greater than unity, and thus these values were suitable for our required configuration. We have also checked the values of equivalent, and maximum shear stresses, which in this case were 4.52 MPa and 2.34 MPa, respectively, and were lower than the yield strength of the core material. All seven parameters showed that the configuration [45 11 / − 45 11 ] 22 , with the core of 440 mm, is safe for our model. The total deformation, in this case, was recorded as 0.024 m, with a total mass of 50,266 kg. When the skin was changed to GFRP, the values of these parameters were 14.99, 13.91, 13.49, and 72.69, respectively. However, the values of equivalent stress and maximum shear stress were increased to 4.46 MPa and 2.31 MPa, respectively. Deformation was increased to −0.028 m, with the same weight of 50,266 kg.
In the case of Paulownia with CFRP sheets under ULS conditions, the readings of MS, SF TW , SF TH , and CF are 2.95, 3.04, 2.95, and 23.43, respectively, for the thickness of [45 10 / − 45 10 ] 20 . The values of equivalent stress and maximum shear stress were lower than Bamboo and equal to 3.75 MPa and 1.94 MPa, and it was less than tensile strength. The mass was reduced to 20,560 kg, for the same value of thickness as compared to the bamboo wood core. This showed that the Paulownia core is relatively better than the bamboo core. However, in this case, the value of deformation is −0.049 m, which is greater than 0.032 m, so its thickness must be increased to satisfy the criteria. In the case of Paulownia core GFRP face skin, the above-mentioned factors were 6.099, 6.22, 5.18, and 40.39, respectively. The deformation was recorded at −0.032 m. The thickness and overall mass were increased to 528 mm and 27,648 kg, respectively. The magnitudes of equivalent stress and maximum shear stress were increased to 2.66 MPa and 1.38 MPa, respectively.
When the Paulownia core was taken with CFRP laminate sheet under SLS conditions, the magnitudes of MS, SF TW , SF TH , and the core factor were 6.88, 7.10, 6.34, and 25.08, respectively. The magnitude of the core factor was greater as compared to other factors. The magnitudes of equivalent stress and maximum shear stress were 3.09 MPa and 1.6 MPa, respectively. Total deformation was increased to −0.038 m for this configuration, which does not satisfy the thickness criterion. When GFRP skin was used, the magnitudes of MS, SF TW , SF TH , and core factor were 11.74, 11.96, 9.97, and 37.81, respectively. The configuration of [45 12 / − 45 12 ] 24 was obtained with a core thickness of 480 mm and an overall thickness of 528 mm, this thickness was greater than the CFRP case. The deformation enhanced to −0.035 m. Equivalent and maximum shear stresses were recorded as 2.66 MPa, and 1.38 MPa, respectively. These values were greater than CFRP face sheets. The total mass was recorded as 27,648 kg.
In the case of Balsa core with CFRP skin, the magnitudes for MS, SF TW , SF TH , and the core factor were 3.44, 3.68, 3.18, and 22.91, respectively. The configuration of [45 14 / − 45 14 ] 28 was obtained, which showed 28 plies on each side were used with the total core thickness of 560 mm. The total thickness increased to the highest value of 616 mm as compared with the previous cases. In this case, 0.039 m of deformation was recorded. The value of equivalent stress and maximum shear stress is 0.61 MPa and 3.47 MPa, respectively, with a total mass of 26,768 kg. When GFRP skin was used, the magnitudes of the above-mentioned constraints were 4.28, 4.72, 3.67, and 26.40, respectively, with the same total mass of 26,768 kg. In this configuration, the bridge's thickness is highest and equals 616 mm with a core thickness of 560 mm. The values of equivalent stresses and maximum shear stresses were 0.6 MPa and 0.35 MPa, respectively.
In the case of CFRP skin and Balsa core under SLS conditions, the magnitudes of MS, SF TW , SF TH , and the core factor were 6.61, 7.08, 6.11, and 22.64, respectively, on the total thickness of 616 mm. In this case, the ply thickness was recorded as 28 mm on either side, and the total weight recorded was 26,768 kg. The value of deformation was −0.039 m; also, equivalent stress and maximum shear stress were recorded as 0.61 MPa and 0.34 MPa, respectively. By using GFRP skin, the values for this configuration were 8.25, 9.08, 7.07, and 26.09, respectively. The deformation was also high, and its value was −0.048 m. The values of equivalent stresses and maximum shear stresses were almost the same as for the CFRP case.

Lay-Up [0/90]
Then the configuration of angle was changed to [0/90], and all the calculations were repeated, and it was shown that significant changes could occur due to the change in angle. For Bamboo wood core and CFRP skin under ULS conditions. The magnitudes for MS, Tsai-Wu (SF TW ), Tsai-Hill (SF TH ), and the core factor criterion were 9.92, 9.94, 9. When Paulownia core and CFRP skin was used, under ULS conditions, the magnitudes of MS, SF TW , SF TH , and core factors were 8.17, 8.47, 8.13, and 24.28, respectively. Core thickness was minimum, and its value was 400 mm. The magnitude of equivalent stress was 1.17 MPa, which is smaller than the [45/−45] alignment. However, the overall mass was decreased to 20,560 kg because the magnitude of thickness was decreased. In the case of GFRP skin, the magnitudes of MS, SF TW , SF TH , the core factor were 7.07, 7.07, 7.08, and 34.73, respectively. The total thickness was greater than the CFRP configuration, and the value was equal to 528 mm, with a core thickness of 480 mm. Deformation was reduced to −0.030 mm, it was −0.035 mm for the [45/−45] skin configuration. The magnitudes of equivalent stress and maximum shear stress were 1.51 MPa and 0.79 MPa, respectively.
In the case of CFRP skin and Paulownia core, under SLS conditions, the magnitudes of MS, SF TW , SF TH , and the core factor were 19.05, 19.87, 18.93, and 25.39, respectively. The deformation was decreased to −0.024 m, as it was −0.038 m, for the [45/−45] configuration. The overall thickness was boosted to 484 mm. Values of equivalent stress and shear stress became small. The weight obtained in this configuration was 22,616 kg. When the GFRP skin was used, the magnitudes of the above-mentioned parameters became 13.64, 13.64, 13.64, and 35.52, respectively. The overall thickness was increased to 528 mm. Deformation was increased to the value of −0.030 m. The values of equivalent stress and maximum shear stress was calculated as 1.5 MPa and 0.79 MPa, respectively.
In the case of CFRP skin and Balsa core, under ULS conditions, the magnitudes of MS, SF TW , SF TH , and the core factor were 9.51, 11.12, 9.46, and 30.79, respectively. All the values were perfect, with a deformation of −0.029 m and a total weight of 22,944 kg with a total thickness of 528 mm. By using GFRP skin, the magnitudes of the parameters were less than CFRP laminate, and their values were 7.37, 7.38, 7.37, and 33.69, respectively. The value of mass was recorded at 26,768 kg. Deformation, equivalent stress, and maximum shear stress values were also increased to −0.034 m, 0.38 MPa, and 0.22 MPa, respectively.
In the case of CFRP skin with Balsa core, under SLS conditions, the magnitudes for MS, SF TW , SF TH , and the core factor were 18.26, 21.37, 18.16, and 30.44, respectively. The total thickness was increased to the value of 528 mm with a CFRP thickness of 24 mm on each side. Deformation, equivalent stress, and maximum shear stress were decreased. By using GFRP skin, the magnitudes of the above-mentioned parameters are 14.21, 14.24, 14.21, and 33.29, respectively. The value of overall thickness was increased to 616 mm, and the total mass reaches to 26,768 kg. Magnitudes of deformation, equivalent stress, and maximum shear stress are −0.034 m, 0.38 MPa, and 0.22 MPa, respectively.

Best Bridge Configuration
Based on the results obtained from simulations, Paulownia has the best configuration for minimum weight and thickness. If angle configuration is considered, then [0/90] has the best results and can achieve the minimum level of deformation in almost all simulations, and if the composite layers are considered, then CFRP layers shows the best results for strength and weight. So, this configuration [0 10 / − 90 10 ] 20 shows the minimum weight and thickness of 20,560 kg and 440 mm, respectively. All the parameters show excellent values of safety factors and stresses under desired loadings. Values for the best case are mentioned in Table 5 on each level of thickness. Figure 2a shows the final values of directional deformation for the Paulownia core. Red color shows the place where the values were maximum. The value was minimum at the middle side of the bridge. Figure 2b shows the values of equivalent stress, the minimum value of 10,667 Pa was recorded on the entire surface, and a maximum value of 1.17 MPa was noticed on the corner sides of the bridge. Figure 2c shows the values of maximum shear stress, 0.62 MPa was recorded on the side corners of the bridge. Figure 2d shows the value safety factor SF TH for Paulownia core, and it is safe for all the values greater than 1. Figure 2e shows the values of a safety factor SF TW .  Figure 2a shows the final values of directional deformation for the Paulownia core. Red color shows the place where the values were maximum. The value was minimum at the middle side of the bridge. Figure 2b shows the values of equivalent stress, the minimum value of 10,667 Pa was recorded on the entire surface, and a maximum value of 1.17 MPa was noticed on the corner sides of the bridge. Figure 2c shows the values of maximum shear stress, 0.62 MPa was recorded on the side corners of the bridge. Figure 2d shows the value safety factor for Paulownia core, and it is safe for all the values greater than 1. Figure 2e shows the values of a safety factor .

Graphical Evaluation and Comparison
Based on increasing thickness, graphs of all the parameters are plotted, as shown in Figure 3. The lay-up [45 10 / − 45 10 ] 20 for the Paulownia core was selected as the best configuration bridge option. For this configuration, there were a total of 40 layers, 20 on either side. Figure 3a-e shows the graphs of all parameters against their thickness.

Graphical Evaluation and Comparison
Based on increasing thickness, graphs of all the parameters are plotted, as shown in Figure 3. The lay-up [45 /−45 ] for the Paulownia core was selected as the best configuration bridge option. For this configuration, there were a total of 40 layers, 20 on either side. Figure 3a-e shows the graphs of all parameters against their thickness.  thickness. (f) Safety factor Tsai-Wu vs. thickness (g) Core factor vs. thickness. Figure 3 shows the effect of increasing length on Design Variables. Total thickness was varied from 44 mm to 616 mm, and the values of different factors were observed. In Figure 3a, when the thickness reached 176 mm, the value of safety factor MS becomes 1, this meant beyond 176 mm all the configurations were safe for safety factor MS. Tsai-Hill is the material constraint, and Figure 3b shows that the value started from 0.07 when the thickness was 44 mm, after that, it gradually increased with thickness and finally became 1 at 176 mm. The graph of Figure 3c comprises three main zones. The values went down more quickly in the first zone. The second zone was between the thickness of 120 mm to 280 mm; the values of the parameters went parallel to the axis in the third zone and the end at the minimum value of 0.32 MPa. Figure 3d shows the equivalent stress, and its value was 118.97 MPa when the thickness was 44 mm. At 132 mm thickness, the value dropped down to 13.05 MPa, and then the trend became parallel to the axis and then finally ended at 0.61 MPa. Figure 3e shows the total deformation, which must be less than 0.032 m. The minimum value to fulfill the criteria was at the thickness of 440 mm. At this point, its value was −0.032 m. Beyond this value, all the configurations are safe, and for our final thickness, the value drops down to −0.012 m. Material constraint Tsai-Wu became 1 at 176 mm thickness in Figure 3f. At a 440 mm thickness, the final value was 16.78. Figure 3g determines the safety of the core, and thus it is known as the core factor. The value was 1 from the starting thickness and became 35.68 at 616 mm thickness. The deformation results obtained from the current research work were compared with the bridge used in a previous study [27].

Conclusions
A composite sandwich structure bridge with wood core was designed based on the minimum thickness and mass. Three different types of woods were used as the core material of the structure. CFRP and GFRP materials were used with two different angle configurations as the skin material of the structure. The FEA model of the bridge was designed in an ACP module with two lanes and two vehicles. Then it was transferred to the static structural system for computing the values of safety factor and other parameters under ULS and SLS conditions. It was concluded that the bridge structure's design and strength greatly depend on the core's fiber orientation and material. After examining the overall results, we concluded that Paulownia wood with [0 /90 ] configuration and  Figure 3 shows the effect of increasing length on Design Variables. Total thickness was varied from 44 mm to 616 mm, and the values of different factors were observed. In Figure 3a, when the thickness reached 176 mm, the value of safety factor MS becomes 1, this meant beyond 176 mm all the configurations were safe for safety factor MS. Tsai-Hill is the material constraint, and Figure 3b shows that the value started from 0.07 when the thickness was 44 mm, after that, it gradually increased with thickness and finally became 1 at 176 mm. The graph of Figure 3c comprises three main zones. The values went down more quickly in the first zone. The second zone was between the thickness of 120 mm to 280 mm; the values of the parameters went parallel to the axis in the third zone and the end at the minimum value of 0.32 MPa. Figure 3d shows the equivalent stress, and its value was 118.97 MPa when the thickness was 44 mm. At 132 mm thickness, the value dropped down to 13.05 MPa, and then the trend became parallel to the axis and then finally ended at 0.61 MPa. Figure 3e shows the total deformation, which must be less than 0.032 m. The minimum value to fulfill the criteria was at the thickness of 440 mm. At this point, its value was −0.032 m. Beyond this value, all the configurations are safe, and for our final thickness, the value drops down to −0.012 m. Material constraint Tsai-Wu became 1 at 176 mm thickness in Figure 3f. At a 440 mm thickness, the final value was 16.78. Figure 3g determines the safety of the core, and thus it is known as the core factor. The value was 1 from the starting thickness and became 35.68 at 616 mm thickness. The deformation results obtained from the current research work were compared with the bridge used in a previous study [27].

Conclusions
A composite sandwich structure bridge with wood core was designed based on the minimum thickness and mass. Three different types of woods were used as the core material of the structure. CFRP and GFRP materials were used with two different angle configurations as the skin material of the structure. The FEA model of the bridge was designed in an ACP module with two lanes and two vehicles. Then it was transferred to the static structural system for computing the values of safety factor and other parameters under ULS and SLS conditions. It was concluded that the bridge structure's design and strength greatly depend on the core's fiber orientation and material. After examining the overall results, we concluded that Paulownia wood with [0 10 /90 10 ] 20 configuration and CFRP layers are the best configurations for minimum weight and thickness. The magnitudes of MS, SF TW , SF TH , and core factor were recorded 8. 17, 8.47, 8.13, and 24.28, respectively. Overall thickness was attained 440 mm with a total mass of 20,560 kg. The values of Equivalent and shear stresses were 1.17 and 0.62 MPa, respectively. Deflection for this case was recorded 32 mm.